this, the major test standards call for wet testing of textile armor.) Mechanisms for this wet loss of performance are not known. Vests that will be tested after ISO-type water immersion tend to have heat-sealed enclosures and those that are tested under NIJ-type water spray methods tend to have water-resistant enclosures. From 2003 to 2005, a large study of the environmental degradation of Zylon armor was undertaken by the US-NIJ. This concluded that water, long-term use, and temperature exposure significantly affect tensile strength and the ballistic performance of PBO or Zylon fiber. This NIJ study on vests returned from the field demonstrated that environmental effects on Zylon resulted in ballistic failures under standard test conditions. Ballistic testing V50 and V0 Measuring the ballistic performance of armor is based on determining the kinetic energy of a bullet at impact. Because the energy of a bullet is a key factor in its penetrating capacity, velocity is used as the primary independent variable in ballistic testing. For most users the key measurement is the velocity at which no bullets will penetrate the armor. Measuring this zero penetration velocity (V0) must take into account variability in armor performance and test variability. Ballistic testing has a number of sources of variability: the armor, test backing materials, bullet, casing, powder, primer and the gun barrel, to name a few. Variability reduces the predictive power of a determination of V0. If, for example, the V0 of an armor design is measured to be with a 9 mm FMJ bullet based on 30 shots, the test is only an estimate of the real V0 of this armor. The problem is variability. If the V0 is tested again with a second group of 30 shots on the same vest design, the result will not be identical. Only a single low velocity penetrating shot is required to reduce the V0 value. The more shots made the lower the V0 will go. In terms of statistics, the zero penetration velocity is the tail end of the distribution curve. If the variability is known and the standard deviation can be calculated, one can rigorously set the V0 at a confidence interval. Test Standards now define how many shots must be used to estimate a V0 for the armor certification. This procedure defines a confidence interval of an estimate of V0. (See "NIJ and HOSDB test methods".) V0 is difficult to measure, so